ASTM-D4832 › Standard Test Method for Preparation and Testing of Controlled Low Strength Material (CLSM) Test Cylinders
Show Complete Document History
The following bibliographic material is provided to assist you with your purchasing decision:
1.1 This test method covers procedures for the preparation, curing, transporting and testing of cylindrical test specimens of controlled low strength material (CLSM) for the determination of compressive strength.
1.2 This test method covers CLSM materials that have a higher strength than the soil but less than 8400 kPa (1200 psi). Typical strengths for most applications fall between 350 to 700 kPa (50 to 100 psi).
1.3 The CLSM used to make the molded specimens shall be sampled after all on-site adjustments have been made to the mixture proportions, including the addition of mix water and any admixtures.
1.4 This test method may be used to prepare and test cylindrical specimens of other mixtures of soil and cementitious materials, such as self-cementing fly ashes.
1.5 CLSM is also known as flowable fill, controlled density fill, soil-cement slurry, soil-cement grout, unshrinkable fill, K-Krete, and other similar names.
1.6 All observed and calculated values shall conform to the guidelines for significant digits and rounding established in Practice .
1.6.1 The procedures used to specify how data are collected/recorded and calculated in this standard are regarded as the industry standard. In addition, they are representative of the significant digits that should generally be retained. The procedures used do not consider material variation, purpose for obtaining the data, special purpose studies, or any considerations for the user’s objectives; and it is common practice to increase or reduce significant digits of reported data to be commensurate with these considerations. It is beyond the scope of this standard to consider significant digits used in analysis methods for engineering design.
1.7 The values stated in SI units are to be regarded as standard. The values given in parentheses after SI units are provided for information only and are not considered standard.
1.7.1 The converted inch-pound units use the gravitational system of units. In this system, the pound (lbf) represents a unit of force (weight), while the unit for mass is slugs. The converted slug unit is not given, unless dynamic (F=ma) calculations are involved.
1.8 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use. See Section .
1.9 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
Significance and Use
5.1 This test method provides standardized requirements for the preparation, curing, transporting and testing of test cylinders of CLSM under field conditions by replicating a “field cure” of the material.
5.1.1 If the cylinders are field cured, as stipulated herein, the resulting compressive strength test data may be used for the following purposes:
18.104.22.168 Acceptance testing for specified strength,
22.214.171.124 Checking the adequacy of mixture proportions for strength,
126.96.36.199 Quality control,
188.8.131.52 Determination of whether the CLSM is capable of being put in service,
184.108.40.206 Adequacy of curing.
5.2 CLSM is typically used as a backfill material around structures, particularly in confined or limited spaces. Compressive strength testing is performed to assist in the design of the mix and to serve as a quality control technique during construction. Mix design is typically based on 28-day strengths and construction control tests performed 7 days after placement. The compressive strength(s) and other test age(s) will vary according to the requirements for the end product. Additional information on the use and history of CLSM is contained in .
5.3 This test is one of a series of quality control tests that can be performed on CLSM during construction to monitor compliance with specification requirements. The other tests that can be used during construction control of CLSM are Practice and Test Methods , , and .
5.4 There are many other combinations of soil, cement, fly ash (cementitious or not), admixtures, water quality or other materials that could be tested using this method. The mixtures will vary depending on the intended use, availability of materials, and placement requirements.
Note 1: The quality of the result produced by this standard is dependent on the competence of the personnel performing it, and the suitability of the equipment and facilities used. Agencies that meet the criteria of Practice are generally considered capable of competent and objective testing/sampling/inspection/and the like. Users of this standard are cautioned that compliance with Practice does not in itself assure reliable results. Reliable results depend on many factors; Practice provides a means of evaluating some of those factors.
backfill; CLSM; compressive strength; construction control; mix design; quality control; soil stabilization;; ICS Number Code 91.100.10 (Cement. Gypsum. Lime. Mortar)
To find similar documents by ASTM Volume:
To find similar documents by classification:
This document comes with our free Notification Service, good for the life of the document.
This document is available in either Paper or PDF format.
April 1, 2018